Creep Deformation in Materials
Academic Resource Center
• Define creep and discuss its importance in
• Identify the primary mechanisms of creep
• Creep model parameters.
• Detail experimental ways to determine creep.
• Discuss design options to minimize creep
Useful concepts revision…
• It is a time- dependent deformation under a
certain applied load.
• Generally occurs at high temperature
(thermal creep), but can also happen at room
temperature in certain materials (e.g. lead or
glass), albeit much slower.
• As a result, the material undergoes a time
dependent increase in length, which could be
dangerous while in service.
Classical Creep Curve
• The rate of deformation is called the creep rate. It
is the slope of the line in a Creep Strain vs. Time
• Primary Creep: starts at a rapid rate and slows with time.
• Secondary Creep: has a relatively uniform rate.
• Tertiary Creep: has an accelerated creep rate and terminates
when the material breaks or ruptures. It is associated with
both necking and formation of grain boundary voids.
Characteristics of Creep
• Creep in service is usually affected by
changing conditions of loading and
• The number of possible stress-temperature-
time combinations is infinite.
• The creep mechanisms is often different
between metals, plastics, rubber, concrete.
• Bulk Diffusion (Nabarro-Herring creep)
• Creep rate decreases as grain size increases
• Grain Boundary Diffusion (Coble creep)
• Stronger grain size dependence than Nabarro Herring
• Dislocation climb/creep
• Controlled by movement of dislocations, strong dependence on applied
• Thermally activated glide
• Occurs in polymers and other viscoelastic materials
• Measures dimensional changes accurately at
constant high temperature and constant load or
• Useful for modeling long term applications which
are strain limited.
• Provides prediction of life expectancy before
service. This is important for example turbine
Creep Test cont’d
• Measures strain vs. time at constant T and
Load (Similar to graph seen previously).
• Relatively low loads and creep rate
• Long duration 2000 to 10,000 hours.
• Not always fracture.
• Strain typically less than 0.5%.
Creep Test cont’d
• Creep generally occurs at elevated
temperatures, so it is common for this type of
testing to be performed with an
environmental chamber for precise
• Temperature control is critical to minimize
the effects of thermal expansion on the
Creep Test: General Procedure
• The unloaded specimen is first heated to the
required T and the gage length is measured.
• The predetermined load is applied quickly
• Measurement of the extension are observed
at frequent interval.
• Average of about 50 readings should be
• To predict the stress and time for long lives
on the basis of much shorter data.
• Plant life 30 to 40 years
• Creep data is usually not available beyond
lives of more than 30000 hrs.
• Larson Miller Parameter and other material
specific models are used.
Larson Miller Parameter
• Model based on Arrhenius rate equation.
LMP= T(C+log tr)
Where T = temperature (K or ºR)
tr = time before failure (hours)
C= material specific constant
• Predicts rupture lives given certain temperature
• First used by General Electric in the 50’s to
perform research on turbine blades.
Stress Rupture Tests
• Determines the time necessary for material to
result in failure under a overload.
• Useful in materials selection where dimensional
tolerances are acceptable, but rupture cannot be
• Generally performed at elevated temperatures.
• Smooth, notched, flat specimens or samples of
any combination can be tested.
Design Considerations to avoid
• Reduce the effect of grain boundaries:
• Use single crystal material with large grains.
• Addition of solid solutions to eliminate vacancies.
• Employ materials of high melting
• Consult Creep Test Data during materials
• Type of service application
• Set adequate inspection intervals according to life
• Abbaschian, Reed-Hill. “Physical Metallurgy
Principles”. 4th edition. 2009
• Dowling, Norman E. Mechanical Behavior of
Materials.3rd edition. 2007
• “Larson Miller Parameter”